1 Types of Strain l a g Engineering Strain: l o l o l b e = l l o l o (a) (b) (c) Shear Strain: FIGURE 2.1 Types of strain. (a) Tensile. (b) Compressive. (c) Shear. All deformation processes in manufacturing involve strains of these types. Tensile strains are involved in stretching sheet metal to make car bodies, compressive strains in forging metals to make turbine disks, and shear strains in making holes by punching. γ = a b
2 Tensile-Test Elastic Stress Plastic Y UTS Y Fracture Offset l o tan -1 E e o e u e f Strain (for l o = 1) l A o l e Original gage length, l o Fracture (a) l f Uniform elongation l u Neck Total elongation l f A f (b) Post-uniform elongation FIGURE 2.2 (a) Original and final shape of a standard tensile-test specimen. (b) Outline of a tensile-test sequence showing different stages in the elongation of the specimen.
3 Mechanical Properties Elongation Poisson s E (GPa) Y (MPa) UTS (MPa) in 5 mm (%) Ratio (ν) METALS (WROUGHT) Aluminum and its alloys Copper and its alloys Lead and its alloys Magnesium and its alloys Molybdenum and its alloys Nickel and its alloys Steels Stainless steels Titanium and its alloys Tungsten and its alloys NONMETALLIC MATERIALS Ceramics Diamond Glass and porcelain Rubbers Thermoplastics Thermoplastics, reinforced Thermosets Boron fibers Carbon fibers Glass fibers (S, E) Kevlar fibers (29, 49, 129) Spectra fibers (9, 1) Note: In the upper table, the lowest values for E, Y, and UTS and the highest values for elongation are for the pure metals. Multiply GPa by 145, to obtain psi, and MPa by 145 to obtain psi. For example 1 GPa = 14,5 ksi, and 1 MPa = 14,5 psi. TABLE 2.1 Typical mechanical properties of various materials at room temperature. See also Tables 1.1, 1.4, 1.8, 11.3 and 11.7.
4 Loading & Unloading; Elongation mm High-purity aluminum-annealed 6 Stress Unload Load Elastic recovery Permanent deformation Strain FIGURE 2.3 Schematic illustration of loading and unloading of a tensile-test specimen. Note that during unloading the curve follows a path parallel to the original elastic slope. Elongation (%) Brass Monel 11-O Aluminum Mild steel Structural silicon steel Magnesium Copper Gage length (in.) FIGURE 2.4 Total elongation in a tensile test as a function of original gage length for various metals. Because necking is a local phenomenon, elongation decreases with gage length. Standard gage length is usually 2 in. (5 mm), although shorter ones can be used if larger specimens are not available.
5 True Stress and True Strain True stress σ = P A True strain ( ) l ε = ln l o = ln ( Ao A ) = ln ( Do D ) 2 = 2ln ( Do D ) TABLE 2.2 Comparison of engineering and true strains in tension e ɛ
6 True Stress - True Strain Curve Fracture True stress K Y f Y = K n Log n 1 1 f True strain ( ) True stress (psi x 1 3 ) 1 1 Y (a) (c) K = 25, Log (b) n = True strain ( ) 1 n FIGURE 2.5 (a) True stress--true strain curve in tension. Note that, unlike in an engineering stress-strain curve, the slope is always positive and that the slope decreases with increasing strain. Although in the elastic range stress and strain are proportional, the total curve can be approximated by the power expression shown. On this curve, Y is the yield stress and Yf is the flow stress. (b) True stresstrue strain curve plotted on a log-log scale. (c) True stress-true strain curve in tension for 11-O aluminum plotted on a log-log scale. Note the large difference in the slopes in the elastic and plastic ranges. Source: After R. M. Caddell and R. Sowerby.
7 Power Law Flow Rule Material K (MPa) n Aluminum, 11-O T O O T O 4.17 Brass, 73, annealed , cold rolled Bronze (phosphor), annealed Cobalt-base alloy, heat treated 27.5 Copper, annealed Molybdenum, annealed Steel, low carbon, annealed hot rolled annealed cold rolled annealed cold rolled annealed P-H, annealed , annealed stainless, annealed stainless, annealed 96.1 Note: 1 MPa = 14,5 psi. Flow rule: σ = Kε n K = Strength coefficient n = Strain hardening exponent TABLE 2.3 Typical values for K and n in Eq at room temperature.
8 True Stress-True Strain for Various Materials Stainless steel 12 True stress (psi x 1 3 ) Brass, as received 865 Steel Brass, annealed 1112 CR Steel 12 Steel Steel 8 Copper, annealed 224-T36 Al O Al O Al 11-O Al H14 Al True strain ( ) MPa FIGURE 2.6 True stress-true strain curves in tension at room temperature for various metals. The point of intersection of each curve at the ordinate is the yield stress Y; thus, the elastic portions of the curves are not indicated. When the K and n values are determined from these curves, they may not agree with those given in Table 2.3 because of the different sources from which they were collected. Source: S. Kalpakjian.
9 Idealized Stress-Strain Curves Stress tan -1 E = EP Y = Y Y = E = Y Strain (a) (b) Y/E (c) Y =Y + E p! tan -1 E p Y E Y + E p ( -Y/E ) True stress K = K n n = 1 < n < 1 n = (d) Y/E (e) 1 True strain (P) FIGURE 2.7 Schematic illustration of various types of idealized stressstrain curves. (a) Perfectly elastic. (b) Rigid, perfectly plastic. (c) Elastic, perfectly plastic. (d) Rigid, linearly strain hardening. (e) Elastic, linearly strain hardening. The broken lines and arrows indicate unloading and reloading during the test. FIGURE 2.8 The effect of strain-hardening exponent n on the shape of true stresstrue strain curves. When n = 1, the material is elastic, and when n =, it is rigid and perfectly plastic.
10 Temperature and Strain Rate Effects Stress (MPa) Stress (psi ) ( C) Elastic modulus Tensile strength Yield strength Elongation Elastic modulus (GPa) Elongation (%) Tensile strength (psi x 1 3 ) C MPa Temperature ( F) Strain rate (s -1 ) FIGURE 2.9 Effect of temperature on mechanical properties of a carbon steel. Most materials display similar temperature sensitivity for elastic modulus, yield strength, ultimate strength, and ductility. FIGURE 2.1 The effect of strain rate on the ultimate tensile strength of aluminum. Note that as temperature increases, the slope increases. Thus, tensile strength becomes more and more sensitive to strain rate as temperature increases. Source: After J. H. Hollomon.
11 Typical Strain Rates in Metalworking Process True Strain Deformation Speed (m/s) Strain Rate (s 1 ) Cold Working Forging, rolling Wire and tube drawing Explosive forming Hot working and warm working Forging, rolling Extrusion Machining Sheet-metal forming Superplastic forming TABLE 2.4 Typical ranges of strain, deformation speed, and strain rates in metalworking processes.
12 Effect on Homologous Temperature.25 Strain rate sensitivity exponent (m) Copper Steel Aluminum 34 Stainless Titanium Rene 41 Mo-T2C Homologous temperature, T T m FIGURE 2.11 Dependence of the strainrate sensitivity exponent m on the homologous temperature T/Tm for various materials. T is the testing temperature and Tm is the melting point of the metal, both on the absolute scale. The transition in the slopes of the curve occurs at about the recrystallization temperature of the metals. Source: After F. W. Boulger.
13 Strain Rate Effects C Material Temperature, C psi 1 3 MPa m Aluminum Aluminum alloys Copper Copper alloys (brasses) Lead Magnesium Steel Low carbon Medium carbon Stainless Titanium Titanium alloys Ti-6Al-4V Zirconium at a strain rate of s 1. Note: As temperature increases, C decreases and m increases. As strain increases, C increases and m may increase or decrease, or it may become negative within certain ranges of temperature and strain. Source: After T. Altan and F.W. Boulger. σ = C ε m C = Strength coefficient m = Strain-rate sensitivity exponent TABLE 2.5 Approximate range of values for C and m in Eq. (2.16) for various annealed metals at true strains ranging from.2 to 1..
14 Effect of Strain Rate Sensitivity on Elongation Total elongation (%) Ti 5A1 2.5Sn Ti 6A1 4V Zircaloy 4 High- and ultra-highcarbon steels Post-uniform elongation (%) A-K Steel HSLA Steel C.R. Aluminum (11) 236-T4 Aluminum 33-O Aluminum 5182-O Aluminum 5182-O Al (15C) 7-3 Brass Zn-Ti Alloy m (a) FIGURE 2.12 (a) The effect of strain-rate sensitivity exponent m on the total elongation for various metals. Note that elongation at high values of m approaches 1%. Source: After D. Lee and W.A. Backofen. (b) The effect of strain-rate sensitivity exponent m on the post uniform (after necking) elongation for various metals. Source: After A.K. Ghosh..2 m (b).4.6
15 Hydrostatic Pressure & Barreling 5 MPa Copper True strain at fracture ( f ) Zinc Magnesium Aluminum Cast iron Hydrostatic pressure (ksi) FIGURE 2.13 The effect of hydrostatic pressure on true strain at fracture in tension for various metals. Even cast iron becomes ductile under high pressure. Source: After H.L.D. Pugh and D. Green. FIGURE 2.14 Barreling in compressing a round solid cylindrical specimen (775-O aluminum) between flat dies. Barreling is caused by friction at the die-specimen interfaces, which retards the free flow of the material. See also Figs.6.1 and 6.2. Source: K.M. Kulkarni and S. Kalpakjian.
16 Plane-Strain Compression Test w > 5h w > 5b b > 2h to 4h h b w Yield stress in plane strain: Y = 2 3 Y = 1.15Y FIGURE 2.15 Schematic illustration of the plane-strain compression test. The dimensional relationships shown should be satisfied for this test to be useful and reproducible. This test gives the yield stress of the material in plane strain, Y. Source: After A. Nadai and H. Ford.
17 Tension & Compression; Baushinger Effect 16 Tension True stress (ksi) Tension Compression 1 5 MPa Y 2Y P True strain ( ) FIGURE 2.16 True stress-true strain curve in tension and compression for aluminum. For ductile metals, the curves for tension and compression are identical. Source: After A.H. Cottrell. Compression FIGURE 2.17 Schematic illustration of the Bauschinger effect. Arrows show loading and unloading paths. Note the decrease in the yield stress in compression after the specimen has been subjected to tension. The same result is obtained if compression is applied first, followed by tension, whereby the yield stress in tension decreases.
18 Disk & Torsion Tests P l r r r t Fracture P σ = 2P πdt FIGURE 2.18 Disk test on a brittle material, showing the direction of loading and the fracture path. This test is useful for brittle materials, such as ceramics and carbides. τ = T 2πr 2 t l FIGURE 2.19 A typical torsion-test specimen. It is mounted between the two heads of a machine and is twisted. Note the shear deformation of an element in the reduced section. r γ = rφ l
19 Simple vs. Pure Shear = (a) (b) FIGURE 2.2 Comparison of (a) simple shear and (b) pure shear. Note that simple shear is equivalent to pure shear plus a rotation.
20 Three- and Four-Point Bend-Tests Maximum bending moment σ = Mc I (a) (b) FIGURE 2.21 Two bend-test methods for brittle materials: (a) threepoint bending; (b) four-point bending. The shaded areas on the beams represent the bending-moment diagrams, described in texts on the mechanics of solids. Note the region of constant maximum bending moment in (b), whereas the maximum bending moment occurs only at the center of the specimen in (a).
21 Hardness Tests Shape of indentation Test Indenter Side view Top view Load, P Hardness number Brinell 1-mm steel or tungsten carbide ball D d d 5 kg 15 kg 3 kg 2P HB = ( D)(D - D 2 - d 2 ) Vickers Diamond pyramid 136 L 1 12 kg HV = 1.854P L 2 b Knoop Diamond pyramid L/b = 7.11 b/t = 4. t L 25 g 5 kg HK = 14.2P L 2 Rockwell A C D B F G E Diamond cone 1 - in. diameter 16 steel ball 1 - in. diameter 8 steel ball 12 t = mm t = mm 6 kg 15 kg 1 kg 1 kg 6 kg 15 kg 1 kg HRA HRC HRD HRB HRF HRG HRE = 1-5t = 13-5t FIGURE 2.22 General characteristics of hardness testing methods. The Knoop test is known as a microhardness test because of the light load and small impressions. Source: After H.W. Hayden, W.G. Moffatt, and V. Wulff.
22 d Hardness Test Considerations d (a) FIGURE 2.23 Indentation geometry for Brinell hardness testing: (a) annealed metal; (b) workhardened metal. Note the difference in metal flow at the periphery of the impressions. (b) Hardness (psi x 1 3 ) MPa Carbon steels, annealed Aluminum, cold worked Carbon steels, cold worked Brinell hardness (kg/mm 2 ) FIGURE 2.25 Bulk deformation in mild steel under a spherical indenter. Note that the depth of the deformed zone is about one order of magnitude larger than the depth of indentation. For a hardness test to be valid, the material should be allowed to fully develop this zone. This is why thinner specimens require smaller indentations. Source: Courtesy of M.C. Shaw and C.T. Yang Yield stress (psi x 1 3 ) FIGURE 2.24 Relation between Brinell hardness and yield stress for aluminum and steels. For comparison, the Brinell hardness (which is always measured in kg/mm 2 ) is converted to psi units on the left scale.
23 Fatigue Stress amplitude, S (MPa) Steel 214-T6 Aluminum alloy Endurance limit psi x Number of cycles, N Number of cycles, N Stress amplitude, S (MPa) Epoxy PTFE (a) (b) Phenolic Diallyl-phthalate Polycarbonate Polysulfone Nylon (dry) psi x 1 3 FIGURE 2.26 Typical S-N curves for two metals. Note that, unlike steel, aluminum does not have an endurance limit..8 MPa FIGURE 2.27 Ratio of fatigue strength to tensile strength for various metals, as a function of tensile strength. Endurance limit/tensile strength Titanium Steels Cast irons Copper alloys.3.2 Cast Aluminum alloys magnesium.1 alloys Wrought magnesium alloys Tensile strength (psi x 1 3 )
24 Creep & Impact Rupture Pendulum Strain Primary Secondary Tertiary Pendulum Specimen (1 x 1 x 55 mm) Specimen (1 x 1 x 75 mm) Notch Instantaneous deformation (a) (b) Time FIGURE 2.28 Schematic illustration of a typical creep curve. The linear segment of the curve (constant slope) is useful in designing components for a specific creep life. FIGURE 2.29 Impact test specimens: (a) Charpy; (b) lzod.
25 Residual Stresses Tensile a b c o Compressive (a) (c) o a d (b) f (d) e FIGURE 2.3 Residual stresses developed in bending a beam made of an elastic, strain-hardening material. Note that unloading is equivalent to applying an equal and opposite moment to the part, as shown in (b). Because of nonuniform deformation, most parts made by plastic deformation processes contain residual stresses. Note that the forces and moments due to residual stresses must be internally balanced.
26 Distortion due to Residual Stress Before After Before After (a) (b) Before After (c) FIGURE 2.31 Distortion of parts with residual stresses after cutting or slitting: (a) rolled sheet or plate; (b) drawn rod; (c) thin-walled tubing. Because of the presence of residual stresses on the surfaces of parts, a round drill may produce an oval-shaped hole because of relaxation of stresses when a portion is removed.
27 Elimination of Residual Stresses Tension Stress Compressive Tensile t c Y c Y t 2Y! c! t Compression (a) (b) (c) (d) FIGURE 2.32 Elimination of residual stresses by stretching. Residual stresses can be also reduced or eliminated by thermal treatments, such as stress relieving or annealing.
28 State of Stress in Metalworking! 1! 1 (a)! 2! 1! 1 (b)! 2! 1! 1! 2! 2 FIGURE 2.33 The state of stress in various metalworking operations. (a) Expansion of a thin-walled spherical shell under internal pressure. (b) Drawing of round rod or wire through a conical die to reduce its diameter; see Section 6.5 (c) Deep drawing of sheet metal with a punch and die to make a cup; see Section 7.6. (c)
29 Strain State in Necking R Correction factor due to Bridgman: Distribution of axial stress a Maximum axial stress Average axial true stress σ σ av = ( 1 + 2R a 1 ) [( 1 + a )] 2R Distribution of radial or tangential stress = True stress in uniaxial tension FIGURE 2.34 Stress distribution in the necked region of a tension-test specimen.
30 States of Stress! 1! 1! 1! 1! 2! 1 (a) (c) (e)! 1! 1! 2 p p (b)! 1 (d) p p (f) p p FIGURE 2.35 Examples of states of stress: (a) plane stress in sheet stretching; there are no stresses acting on the surfaces of the sheet. (b) plane stress in compression; there are no stresses acting on the sides of the specimen being compressed. (c) plane strain in tension; the width of the sheet remains constant while being stretched. (d) plane strain in compression (see also Fig. 2.15); the width of the specimen remains constant due to the restraint by the groove. (e) Triaxial tensile stresses acting on an element. (f) Hydrostatic compression of an element. Note also that an element on the cylindrical portion of a thin-walled tube in torsion is in the condition of both plane stress and plane strain (see also Section ).
31 Yield Criteria Compression Tension!! 1! 1 1!1 Y Maximum-shear Y stress criterion! 1 Tension Distortion-energy criterion Maximum-shear-stress criterion: σ max σ min = Y Distortion-energy criterion:! 1!! 1 Compression 1! 1 (σ 1 σ 2 ) 2 + (σ 2 σ 3 ) 2 + (σ 3 σ 1 ) 2 = 2Y 2 FIGURE 2.36 Plane-stress diagrams for maximum -shear-stress and distortion-energy criteria. Note that 2 =.
32 Flow Stress and Work of Deformation True stress Y f Y Y u 1 Flow stress: Ȳ = Kεn 1 n + 1 True strain (!) FIGURE 2.37 Schematic illustration of true stress-true strain curve showing yield stress Y, average flow stress, specific energy u1 and flow stress Yf.! 1 Specific energy u = Z ε σd ε
33 Ideal & Redundant Work (a) Total specific energy: u total = u ideal + u f riction + u redundant (b) (c) FIGURE 2.38 Deformation of grid patterns in a workpiece: (a) original pattern; (b) after ideal deformation; (c) after inhomogeneous deformation, requiring redundant work of deformation. Note that (c) is basically (b) with additional shearing, especially at the outer layers. Thus (c) requires greater work of deformation than (b). See also Figs. 6.3 and Efficiency: η = u ideal u total
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
Plastic Behaviour - Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hot-rolled, cold-rolled, heat treated, etc.).
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a free-body diagram),
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stress-strain diagram Mild steel : proportional stage, elastic limit, yielding
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B-306) INTRODUCTION TENSION TEST Mechanical testing
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
1 Unit 6: EXTRUSION Introduction: Extrusion is a metal working process in which cross section of metal is reduced by forcing the metal through a die orifice under high pressure. It is used to produce cylindrical
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
Laboratory 2 Hardness Testing Objectives Students are required to understand the principles of hardness testing, i.e., Rockwell, Brinell and Vickers hardness tests. Students are able to explain variations
Hardness Test Chapter 9 Subjects of interest Introduction/objectives Brinell hardness Meyer hardness Vickers hardness Rockwell hardness Microhardness tests Relationship between hardness and the flow curve
5. MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS Samples of engineering materials are subjected to a wide variety of mechanical tests to measure their strength, elastic constants, and other material
Training Objective After watching the program and reviewing this printed material, the viewer will become familiar with further aspects of tool design by exploring the materials used in toolmaking. Tool
Example: 1 A 300-mm-wide strip 25 mm thick is fed through a rolling mill with two powered rolls each of radius = 250 mm. The work thickness is to be reduced to 22 mm in one pass at a roll speed of 50 rev/min.
PLASTIC DEFORMATION AND STRESS-STRAIN CURVES Introduction Background Unit: Plastic Deformation and Stress-Strain Curves In the last unit we studied the elastic response of materials to externally applied
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
Mechanics of Materials-Steel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, Jan-Feb 2016, pp. 119-130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
Experiment: Mechanical Testing- Impact & Hardness Testing Objective The main objective of this experiment is to introduce two important basic mechanical property tests; hardness (using Rockwell testing)
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for soda-lime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
Chapter 7: Fatigue and Impact All machine and structural designs are problems in fatigue because the forces of Nature are always at work and each object must respond in some fashion. Carl Osgood, Fatigue
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
1 Lecture 1. Material Properties 1. Background Manufacturing is the process of converting some material into a part or product. It is the most fundamental activity in any civilization. Everything around
Lecture slides on rolling By: Dr H N Dhakal Lecturer in Mechanical and Marine Engineering, School of Engineering, University of Plymouth Bulk deformation forming (rolling) Rolling is the process of reducing
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 2322-5009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277-284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
3 Mechanical Properties 3 1 Tensile Strength The -strain curve when tension is applied to ASTM-D638 type 1 test piece of Iupilon / NOVAREX at a strain velocity of 5mm/min is shown in Fig. 3 1 1. The following
T dition CHTR MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University Stress and Strain xial oading - Contents Stress & Strain: xial oading
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
s 410, 420, 425 Mod, and 440A GENERAL PROPERTIES s 410, 420, 425 Modified, and 440A (see composition on Page 2) are hardenable, straight-chromium stainless steels which combine superior wear resistance
RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE Ali Fatemi-University of Toledo All Rights Reserved Chapter 8 Residual Stresses & Their Effects 1 RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE
NOTCHES AND THEIR EFFECTS Ali Fatemi - University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations S-N Approach for Notched Members
Engineering Material Ferrous material; A general classification of engineering materials is shown in Figure 1.8. Engineering material can be broadly classified as Metallic and Non-Metallic materials. The
Sheet metal operations - Bending and related processes R. Chandramouli Associate Dean-Research SASTRA University, Thanjavur-613 401 Table of Contents 1.Quiz-Key... Error! Bookmark not defined. 1.Bending
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
ME 354, MECHANICS OF MATERIALS LABORATORY 01 Januarly 2000 / mgj MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS: HARDNESS TESTING* PURPOSE The purpose of this exercise is to obtain a number of experimental
METALLURGY AND FOUNDRY ENGINEERING Vol. 33, 2007, No. 1 Jerzy Kajtoch * STRAIN IN THE UPSETTING PROCESS 1. INTRODUCTION Upsetting is an technological operation of open die forging, which is performed in
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
ATI 316Ti Stainless Steel: Austenitic (UNS S31635) GENERAL PROPERTIES ATI 316Ti stainless is a titanium-stabilized version of Type 316 molybdenum-bearing austenitic stainless steel. It is also known as
STRESS-STRAIN CURVES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 August 23, 2001 Introduction Stress-strain curves are an extremely
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
Homework solutions for test 2 HW for Lecture 7 22.2 What is meant by the term faying surface? Answer. The faying surfaces are the contacting surfaces in a welded joint. 22.3 Define the term fusion weld.
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0 - INTRODUCTION See General Lab Report Format
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
Typical stress-strain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A = --- A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
Technical Data BLUE SHEET Allegheny Ludlum Corporation Pittsburgh, PA Martensitic Stainless Steels Types 410, 420, 425 Mod, and 440A GENERAL PROPERTIES Allegheny Ludlum Types 410, 420, 425 Modified, and
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
Material Science Engineering and Steel Making/Metallurgy Stark County High Schools 2016 Agenda What is Material Science Engineering Basics of Steel Making Steel Processing and Properties 2 What is Material
ALLOY 800 / 800H / 800AT DATA SHEET UNS N08800 / UNS N08801 / UNS N08811 GENERAL PROPERTIES ////////////////////////////////////////////////////// //// 800 (UNS N08800), 800H (UNS N08810) and 800AT (UNS
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
Mr. Patrick J Camilleri B.Ed (Hons) M.Ed Science (Sheffield) Department of Physics JC Malta Properties of Matter Basics You Should Know Elasticity. Young modulus 1. Hooke's law. Extension α tension (force
Designation: E 40 02 Standard Conversion Tables for Metals Relationship Among Brinell,, Rockwell, Superficial, Knoop, and Scleroscope This standard is issued under the fixed designation E 40; the number
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
CHAPTER1 Fundamentals of Extrusion The first chapter of this book discusses the fundamentals of extrusion technology, including extrusion principles, processes, mechanics, and variables and their effects
Superior performance Co-Ni Alloy Product (SPRON) Product Catalogue 21 211 Superior performance Co-Ni Alloy Product (SPRON) solves designers problems " " is a special metal (Co-Ni alloy) developed for mechanical
Mechanical Properties and Fracture Analysis of Glass David Dutt Chromaglass, Inc. IES ALC Williamsburg 2006 2 IES ALC Williamsburg 2006 3 Outline The Ideal The Practical The Reality IES ALC Williamsburg
Metallurgy Made Simple Section II Metal Identification Titanium Nickel Copper Cast Iron 25 Greystone Drive Suite 7 Lynchburg, Virginia 24502 firstname.lastname@example.org ..... There are several Metal Identification
DIE CASTING ALLOYS A wide variety of die casting alloys, a mixture of two or more metals, are available with a comprehensive range of physical and mechanical properties for almost any application a designer
1 Introduction to Hardness Testing Hardness has a variety of meanings. To the metals industry, it may be thought of as resistance to permanent deformation. To the metallurgist, it means resistance to penetration.
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1 - LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
FAILURE MODES and MATERIALS PROPERTIES MECH2300 - Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
PAGE 1/10 1 Density The density of optical glass varies from 239 for N-BK10 to 603 for SF66 In most cases glasses with higher densities also have higher refractive indices (eg SF type glasses) The density
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
ITU Department of Mechanical Engineering MANUFACTURING PROPERTIES of ENGINEERING MATERIALS Lecture Notes Prof.Dr.Ahmet Aran 2007 CONTENTS 1. Engineering Materials and Their Properties 1.1. Classification
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip